LMucko/crystallography-open-database huggingface dataset:
Paravinogradovite, (Na,_)2[(Ti,Fe)4{Si2O6}2{Si3AlO10}(OH)4]H2O, a new mineral species from the Khibina Alkaline Massif, Kola Penninsula, Russia: Description and crystal structure Locality: Khibina Alkaline Massif, Kola Penninsula, Russia
Khomyakov, A. P.; Kulikova, I. E.; Sokolova, E. V.; Hawthorne, F. C.; Kartashov, P. M.; The Canadian Mineralogist 41 (2003) 989–1002; doi:10.2113/gscanmin.41.4.989

data_9004787
_publ_section_title
;Paravinogradovite, (Na,_)2[(Ti,Fe)4{Si2O6}2{Si3AlO10}(OH)4]H2O, a new mineral
 species from the Khibina Alkaline Massif, Kola Penninsula, Russia:
 Description and crystal structure Locality: Khibina Alkaline Massif, Kola
 Penninsula, Russia
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              989
_journal_page_last               1002
_journal_paper_doi               10.2113/gscanmin.41.4.989
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source
'Khibina Alkaline Massif, Kola Penninsula, Russia'
_chemical_formula_sum
'Al0.1 Be0.3 Fe0.48 H10 K0.13 Na2.07 O27.17 Si7.6 Ti3.52'
_chemical_name_mineral           Paravinogradovite
_space_group_IT_number           1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_cell_angle_alpha                70.466
_cell_angle_beta                 78.472
_cell_angle_gamma                89.932
_cell_formula_units_Z            1
_cell_length_a                   5.2533
_cell_length_b                   8.7411
_cell_length_c                   12.9480
_cell_volume                     547.653
_database_code_amcsd             0005880
_exptl_crystal_density_diffrn    2.764
_cod_original_cell_volume        547.654
_cod_original_formula_sum
'Na2.07 K.13 (Ti3.52 Fe.48) Si7.6 Al.1 Be.3 O27.17 H10'
_cod_database_code               9004787
The crystal structure of orlandiite, Pb3Cl4(SeO3).H2O, a complex case of twinning and disorder
Demartin, F.; Gramaccioli, C. M.; Pilati, T.; The Canadian Mineralogist 41 (2003) 1147–1153; doi:10.2113/gscanmin.41.5.1147

data_9004788
_publ_section_title
;
 The crystal structure of orlandiite, Pb3Cl4(SeO3).H2O, a complex case
 of twinning and disorder
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1147
_journal_page_last               1153
_journal_paper_doi               10.2113/gscanmin.41.5.1147
_journal_volume                  41
_journal_year                    2003
_chemical_formula_sum            'Cl2 H O2 Pb1.5 Se0.5'
_chemical_name_mineral           Orlandiite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                62.58
_cell_angle_beta                 71.84
_cell_angle_gamma                75.13
_cell_formula_units_Z            4
_cell_length_a                   8.136
_cell_length_b                   8.430
_cell_length_c                   9.233
_cell_volume                     529.293
_database_code_amcsd             0005881
_exptl_crystal_density_diffrn    5.700
_cod_original_formula_sum        'Pb1.5 Se.5 Cl2 O2 H'
_cod_database_code               9004788
Kupcikite, Cu3.4Fe0.6Bi5S10, a new Cu-Bi sulfosalt from Felbertal, Austria, and its crystal structure
Topa, D.; Makovicky, E.; Balic-Zunic T; Paar, W. H.; The Canadian Mineralogist 41 (2003) 1155–1166; doi:10.2113/gscanmin.41.5.1155

data_9004789
_publ_section_title
;
 Kupcikite, Cu3.4Fe0.6Bi5S10, a new Cu-Bi sulfosalt from
 Felbertal, Austria, and its crystal structure
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1155
_journal_page_last               1166
_journal_paper_doi               10.2113/gscanmin.41.5.1155
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Felbertal, Austria'
_chemical_formula_sum            'Bi5 Cu3.42 Fe0.58 S10'
_chemical_name_mineral           Kupcikite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 108.56
_cell_angle_gamma                90
_cell_length_a                   17.512
_cell_length_b                   3.9103
_cell_length_c                   12.869
_cell_formula_units_Z            2
_cell_volume                     835.401
_database_code_amcsd             0005882
_exptl_crystal_density_diffrn    6.421
_cod_original_formula_sum        'Cu3.42 Fe.58 Bi5 S10'
_cod_database_code               9004789
The crystal structure of vasilyevite, (Hg2)10O6I3(Br,Cl)3(CO3)
Cooper, M. A.; Hawthorne, F. C.; The Canadian Mineralogist 41 (2003) 1173–1181; doi:10.2113/gscanmin.41.5.1173

data_9004790
_publ_section_title
;
 The crystal structure of vasilyevite, (Hg2)10O6I3(Br,Cl)3(CO3)
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1173
_journal_page_last               1181
_journal_paper_doi               10.2113/gscanmin.41.5.1173
_journal_volume                  41
_journal_year                    2003
_chemical_formula_sum            'C0.85 Br1.64 Cl1.36 Hg20 I3 O8.55 S0.15'
_chemical_name_mineral           Vasilyevite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                93.262
_cell_angle_beta                 90.548
_cell_angle_gamma                115.422
_cell_length_a                   9.344
_cell_length_b                   10.653
_cell_length_c                   18.265
_cell_formula_units_Z            2
_cell_volume                     1638.254
_database_code_amcsd             0005883
_exptl_crystal_density_diffrn    9.576
_cod_original_formula_sum        'Hg20 (C.85 S.15) O8.55 I3 (Br1.64 Cl1.36)'
_cod_database_code               9004790
The crystal structure of seidite-(Ce), Na4(Ce,Sr)2{Ti(OH)2(Si8O18)}(O,OH,F)4.5H2O, a modular microporous titanosilicate of the rhodesite group
Ferraris, G.; Belluso, E.; Gula, A.; Soboleva, S. V.; Khomyakov, A. P.; The Canadian Mineralogist 41 (2003) 1183–1192; doi:10.2113/gscanmin.41.5.1183

data_9004791
_publ_section_title
;The crystal structure of seidite-(Ce),
 Na4(Ce,Sr)2{Ti(OH)2(Si8O18)}(O,OH,F)4.5H2O, a modular microporous
 titanosilicate of the rhodesite group
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1183
_journal_page_last               1192
_journal_paper_doi               10.2113/gscanmin.41.5.1183
_journal_volume                  41
_journal_year                    2003
_chemical_formula_sum
;Ba0.12 Ca0.2 Ce0.42 F0.84 Fe0.02 H12.8 K0.28 La0.3 Mn0.05 Na3.2 Nb0.06 Nd0.1
 O28.02 Pr0.04 Si8 Sm0.02 Sr0.54 Th0.12 Ti0.86
;
_chemical_name_mineral           Seidite-(Ce)
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.6
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   24.61
_cell_length_b                   7.23
_cell_length_c                   14.53
_cell_volume                     2577.000
_database_code_amcsd             0005884
_exptl_crystal_density_diffrn    2.733
_cod_original_formula_sum
;Si8 Ti.86 Nb.06 Mn.05 Fe.02 Ce.42 La.3 Nd.1 Pr.04 Sm.02 Sr.54 Ca.2 Th.12
 Na3.2 K.28 Ba.12 O28.02 F.84 H12.8
;
_cod_database_code               9004791
The crystal chemistry of shcherbakovite from the Khibina Massif, Kola Peninsula, Russia Locality: Khibina Massif, Kola Peninsula, Russia
Uvarova, Y. A.; Sokolova, E. V.; Hawthorne, F. C.; Liferovich, R. P.; Mitchell, R. H.; The Canadian Mineralogist 41 (2003) 1193–1201; doi:10.2113/gscanmin.41.5.1193

data_9004792
_publ_section_title
;The crystal chemistry of shcherbakovite from the Khibina Massif, Kola
 Peninsula, Russia Locality: Khibina Massif, Kola Peninsula, Russia
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1193
_journal_page_last               1201
_journal_paper_doi               10.2113/gscanmin.41.5.1193
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Khibina Massif, Kola Peninsula, Russia'
_chemical_formula_sum
'Ba0.23 Ca0.02 Fe0.08 H0.48 K1.66 Na1.07 Nb0.48 O14 Si4 Ti1.4 Zr0.04'
_chemical_name_mineral           Shcherbakovite
_space_group_IT_number           74
_symmetry_space_group_name_Hall  '-I 2b 2'
_symmetry_space_group_name_H-M   'I m m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.1538
_cell_length_b                   10.5569
_cell_length_c                   13.9882
_cell_volume                     1204.088
_database_code_amcsd             0005885
_exptl_crystal_density_diffrn    3.191
_cod_original_formula_sum
'K1.66 Ba.23 Na1.07 Ca.02 Ti1.4 Nb.48 Fe.08 Zr.04 Si4 O14 H.48'
_cod_database_code               9004792
Crystal chemistry of the rosenbuschite group Sample: WBC-13
Christiansen, C. C.; Johnsen, O.; Makovicky, E.; The Canadian Mineralogist 41 (2003) 1203–1224; doi:10.2113/gscanmin.41.5.1203

data_9004793
_publ_section_title
;
 Crystal chemistry of the rosenbuschite group
 Sample: WBC-13
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1203
_journal_page_last               1224
_journal_paper_doi               10.2113/gscanmin.41.5.1203
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Werner Bjerge, East Greenland'
_chemical_formula_sum
'Ca4.91 Ce0.25 F3 Fe0.05 Mn0.11 Na1.59 Nb0.03 O15 Si4 Ti0.92 Y0.06 Zr0.09'
_chemical_name_mineral           Gotzenite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                89.921
_cell_angle_beta                 101.132
_cell_angle_gamma                100.639
_cell_formula_units_Z            1
_cell_length_a                   9.6192
_cell_length_b                   5.7249
_cell_length_c                   7.3307
_cell_volume                     389.044
_database_code_amcsd             0005886
_exptl_crystal_density_diffrn    3.188
_cod_original_formula_sum
'Ca4.91 Ce.25 Mn.11 Zr.09 Y.06 Na1.59 (Ti.92 Fe.05 Nb.03) Si4 O15 F3'
_cod_database_code               9004793
Crystal chemistry of the rosenbuschite group Sample: LF-A5
Christiansen, C. C.; Johnsen, O.; Makovicky, E.; The Canadian Mineralogist 41 (2003) 1203–1224; doi:10.2113/gscanmin.41.5.1203

data_9004794
_publ_section_title
;
 Crystal chemistry of the rosenbuschite group
 Sample: LF-A5
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1203
_journal_page_last               1224
_journal_paper_doi               10.2113/gscanmin.41.5.1203
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Langesund Fjord, Norway'
_chemical_formula_sum
;Ca7.905 Ce0.03 F6.04 Fe0.11 Hf0.04 Mn0.22 Na3.975 Nb0.17 O29.96 Si8 Ti0.95
 Y0.15 Zr2.45
;
_chemical_name_mineral           Rosenbuschite
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                90.216
_cell_angle_beta                 100.308
_cell_angle_gamma                111.868
_cell_formula_units_Z            1
_cell_length_a                   10.137
_cell_length_b                   11.398
_cell_length_c                   7.2714
_cell_volume                     764.826
_database_code_amcsd             0005887
_exptl_crystal_density_diffrn    3.375
_cod_original_formula_sum
;Zr2.45 Ca7.905 Hf.04 Mn.22 Y.15 Ce.03 Na3.975 Ti.95 Nb.17 Fe.11 Si8 O29.96
 F6.04
;
_cod_database_code               9004794
Crystal chemistry of the rosenbuschite group Sample: 1993.158
Christiansen, C. C.; Johnsen, O.; Makovicky, E.; The Canadian Mineralogist 41 (2003) 1203–1224; doi:10.2113/gscanmin.41.5.1203

data_9004795
_publ_section_title
;
 Crystal chemistry of the rosenbuschite group
 Sample: 1993.158
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1203
_journal_page_last               1224
_journal_paper_doi               10.2113/gscanmin.41.5.1203
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Lovozero Complex, Kola Peninsula, Russia'
_chemical_formula_sum
'Ca0.26 F3 Fe0.32 Mg0.305 Mn0.425 Na3.91 Nb0.04 O15 Si4 Ti1.36 Zr1.38'
_chemical_name_mineral           Seidozerite
_space_group_IT_number           13
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 102.713
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.5558
_cell_length_b                   7.0752
_cell_length_c                   18.406
_cell_volume                     705.773
_database_code_amcsd             0005888
_exptl_crystal_density_diffrn    3.543
_cod_original_formula_sum
'Zr1.38 Ti1.36 Fe.32 Mg.305 Nb.04 Mn.425 Ca.26 Na3.91 Si4 O15 F3'
_cod_database_code               9004795
Crystal chemistry of uranyl molybdates. IX. A novel uranyl molybdate sheet in the structure of Tl2[(UO2)2O(MoO5)]
Krivovichev, S. V.; Burns, P. C.; The Canadian Mineralogist 41 (2003) 1225–1231; doi:10.2113/gscanmin.41.5.1225

data_9004796
_publ_section_title
;Crystal chemistry of uranyl molybdates. IX. A novel uranyl molybdate sheet in
 the structure of Tl2[(UO2)2O(MoO5)]
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1225
_journal_page_last               1231
_journal_paper_doi               10.2113/gscanmin.41.5.1225
_journal_volume                  41
_journal_year                    2003
_chemical_formula_structural     Tl2[(UO2)2O(MoO5)]
_chemical_formula_sum            'Mo2 O20 Tl4 U4'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.122
_cell_angle_gamma                90
_cell_length_a                   8.2527
_cell_length_b                   28.5081
_cell_length_c                   9.1555
_cell_formula_units_Z            4
_cell_volume                     2088.906
_database_code_amcsd             0005889
_exptl_crystal_density_diffrn    7.255
_cod_original_formula_sum        'U4 Tl4 Mo2 O20'
_cod_database_code               9004796
_amcsd_formula_title             Tl2[(UO2)2O(MoO5)]
Sodic-ferri-ferropedrizite and ferri-clinoferroholmquistite: mineral data and degree of order of the A-site cations in Li-rich amphiboles Sequence number in the CNR-IGG database: SEQ 1039
Oberti, R.; Camara, F.; Caballero, J. M.; Ottolini, L.; The Canadian Mineralogist 41 (2003) 1345–1354; doi:10.2113/gscanmin.41.6.1345

data_9004797
_publ_section_title
;Sodic-ferri-ferropedrizite and ferri-clinoferroholmquistite: mineral data and
 degree of order of the A-site cations in Li-rich amphiboles Sequence number
 in the CNR-IGG database: SEQ 1039
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1345
_journal_page_last               1354
_journal_paper_doi               10.2113/gscanmin.41.6.1345
_journal_volume                  41
_journal_year                    2003
_chemical_formula_sum
;Al0.22 Ca0.04 F0.56 Fe3.26 H1.44 K0.06 Li1.87 Mg Mn0.35 Na1.2 O23.44 Si8
 Ti0.12
;
_chemical_name_mineral           Sodic-ferri-ferropedrizite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 102.06
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.496
_cell_length_b                   17.883
_cell_length_c                   5.297
_cell_volume                     879.667
_database_code_amcsd             0005890
_exptl_crystal_density_diffrn    3.374
_cod_original_formula_sum
'Na1.2 K.06 Fe3.26 Ca.04 Li1.87 Mg Al.22 Ti.12 Mn.35 Si8 O23.44 F.56 H1.44'
_cod_database_code               9004797
Sodic-ferri-ferropedrizite and ferri-clinoferroholmquistite: mineral data and degree of order of the A-site cations in Li-rich amphiboles Sequence number in the CNR-IGG database: SEQ 1043
Oberti, R.; Camara, F.; Caballero, J. M.; Ottolini, L.; The Canadian Mineralogist 41 (2003) 1345–1354; doi:10.2113/gscanmin.41.6.1345

data_9004798
_publ_section_title
;Sodic-ferri-ferropedrizite and ferri-clinoferroholmquistite: mineral data and
 degree of order of the A-site cations in Li-rich amphiboles Sequence number
 in the CNR-IGG database: SEQ 1043
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1345
_journal_page_last               1354
_journal_paper_doi               10.2113/gscanmin.41.6.1345
_journal_volume                  41
_journal_year                    2003
_chemical_formula_sum
'Al0.26 Ca0.02 F0.2 Fe3.24 H1.8 Li2.18 Mg1.06 Mn0.14 Na0.64 O23.8 Si8 Zn0.02'
_chemical_name_mineral           Ferri-clinoferroholmquistite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 101.88
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.462
_cell_length_b                   17.898
_cell_length_c                   5.302
_cell_volume                     878.666
_database_code_amcsd             0005891
_exptl_crystal_density_diffrn    3.267
_cod_original_formula_sum
'Na.64 Li2.18 Ca.02 Mg1.06 Fe3.24 Al.26 Zn.02 Mn.14 Si8 O23.8 F.2 H1.8'
_cod_database_code               9004798
Disordered Mg-bearing olenite from a granitic pegmatite at Goslarn, Austria: A chemical, structural, and infrared spectroscopic study Sample: GOS1, from the sample rim
Ertl, A.; Hughes, J. M.; Brandstatter, F.; Dyar, M. D.; Prasad, P. S. R.; The Canadian Mineralogist 41 (2003) 1363–1370; doi:10.2113/gscanmin.41.6.1363

data_9004799
_publ_section_title
;
 Disordered Mg-bearing olenite from a granitic pegmatite at Goslarn, Austria:
 A chemical, structural, and infrared spectroscopic study
 Sample: GOS1, from the sample rim
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1363
_journal_page_last               1370
_journal_paper_doi               10.2113/gscanmin.41.6.1363
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Goslarn, Austria'
_chemical_formula_sum
;Al6.405 B3 Ca0.1 F0.03 Fe0.39 H3.05 K0.001 Mg2.163 Na0.71 O30.97 Si5.952
 Ti0.09
;
_chemical_name_mineral           Olenite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   15.9238
_cell_length_b                   15.9238
_cell_length_c                   7.1822
_cell_volume                     1577.181
_database_code_amcsd             0005892
_exptl_crystal_density_diffrn    3.066
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
'Na.71 Ca.1 K.001 Al6.405 Mg2.163 Fe.39 Ti.09 Si5.952 B3 O30.97 F.03 H3.05'
_cod_database_code               9004799
Disordered Mg-bearing olenite from a granitic pegmatite at Goslarn, Austria: A chemical, structural, and infrared spectroscopic study Sample: GOS2, from the sample core
Ertl, A.; Hughes, J. M.; Brandstatter, F.; Dyar, M. D.; Prasad, P. S. R.; The Canadian Mineralogist 41 (2003) 1363–1370; doi:10.2113/gscanmin.41.6.1363

data_9004800
_publ_section_title
;
 Disordered Mg-bearing olenite from a granitic pegmatite at Goslarn, Austria:
 A chemical, structural, and infrared spectroscopic study
 Sample: GOS2, from the sample core
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1363
_journal_page_last               1370
_journal_paper_doi               10.2113/gscanmin.41.6.1363
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Goslarn, Austria'
_chemical_formula_sum
;Al6.483 B3 Ca0.11 F0.03 Fe0.411 H3.07 K0.002 Mg2.007 Na0.64 O30.97 Si6
 Ti0.099
;
_chemical_name_mineral           Olenite
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   15.9149
_cell_length_b                   15.9149
_cell_length_c                   7.1757
_cell_volume                     1573.993
_database_code_amcsd             0005893
_exptl_crystal_density_diffrn    3.072
_cod_original_sg_symbol_H-M      'R 3 m'
_cod_original_formula_sum
'Na.64 Ca.11 K.002 Al6.483 Mg2.007 Fe.411 Ti.099 Si6 B3 O30.97 F.03 H3.07'
_cod_database_code               9004800
Fluorvesuvianite, Ca19(Al,Mg,Fe)13[SiO4]10[Si2O7]4O(F,OH)9, a new mineral species from Pitkaranta, Karelia, Russia: Description and crystal structure
Britvin, S. N.; Antonov, A. A.; Krivovichev, S. V.; Armbruster, T.; Burns, P. C.; Chukanov, N. V.; The Canadian Mineralogist 41 (2003) 1371–1380; doi:10.2113/gscanmin.41.6.1371

data_9004801
_publ_section_title
;Fluorvesuvianite, Ca19(Al,Mg,Fe)13[SiO4]10[Si2O7]4O(F,OH)9, a new mineral
 species from Pitkaranta, Karelia, Russia: Description and crystal structure
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              1371
_journal_page_last               1380
_journal_paper_doi               10.2113/gscanmin.41.6.1371
_journal_volume                  41
_journal_year                    2003
_chemical_compound_source        'Pitkaranta, Karelia, Russia'
_chemical_formula_sum
'Al10.24 Ca19 F5.76 Fe1.368 H Mg1.36 O72.24 Si17.606'
_chemical_name_mineral           Fluorvesuvianite
_space_group_IT_number           126
_symmetry_space_group_name_Hall  '-P 4a 2bc'
_symmetry_space_group_name_H-M   'P 4/n n c :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   15.5295
_cell_length_b                   15.5295
_cell_length_c                   11.7808
_cell_formula_units_Z            2
_cell_volume                     2841.121
_database_code_amcsd             0005894
_exptl_crystal_density_diffrn    3.399
_cod_original_sg_symbol_H-M      'P 4/n n c'
_cod_original_formula_sum
'Si17.606 Ca19 Fe1.368 Al10.24 Mg1.36 O72.24 F5.76 H'
_cod_database_code               9004801